|Year : 2015 | Volume
| Issue : 6 | Page : 627-632
|Histological analysis of the biocompatibility of calcium hydroxide associated with a new vehicle
Jacy Simi Junior1, Ricardo Machado2, Cássio José Alves de Souza3, Adriano Motta Loyola4, Luiz Pascoal Vansan5, João Humberto Antoniazzi6
1 Department of Endodontics, North of Minas Gerais Integrated College - FUNORTE/SOEBRÁS, Florianópolis, Santa Catarina, Brazil
2 Department of Multidisciplinary Clinic I and II (Endodontics), Paranaense University - UNIPAR, Francisco Beltrão, Paraná, Brazil
3 Department of Endodontics, Federal University of Uberlândia - UFU, Uberlândia, Minas Gerais, Brazil
4 Department of Pathology, Federal University of Uberlândia - UFU, Uberlândia, Minas Gerais, Brazil
5 Department of Restorative Dentistry (Endodontics), Ribeirão Preto Dental School, University of São Paulo - FORP/USP, Ribeirão Preto, São Paulo, Brazil
6 Department of Endodontics, University of São Paulo - USP/SP, São Paulo, Brazil
Click here for correspondence address and email
|Date of Submission||26-Jan-2015|
|Date of Decision||12-Jul-2015|
|Date of Acceptance||01-Feb-2016|
|Date of Web Publication||18-Feb-2016|
| Abstract|| |
Background: Several substances have been researched to act as vehicles associated with calcium hydroxide. The specific type of vehicle is directly related to the effectiveness of the ionic dissociation, antimicrobial action, and biocompatibility of this medication.
Aim: To make a histological evaluation of the biocompatibility of calcium hydroxide associated with a new vehicle (triethanolamine), compared with polyethylene glycol, saline solution, and olive oil.
Materials and Methods: Fifty mice of guinea pig species were randomly divided into five groups (n = 10) according to each vehicle used - Group 1: calcium hydroxide, Group 2: triethanolamine, Group 3: polyethylene glycol, Group 4: saline solution, and Group 5: olive oil - and further divided into subgroups according to the two analysis periods - (a) 30 and (b) 90 days. Teflon carriers filled with the evaluated substances were placed in standardized bone cavities in the anterior mandible region. The animals were euthanized to perform a histological analysis after the time periods analyzed.
Results: In 30 days, specimens from Groups 1, 3, and 5 showed a very pronounced inflammatory response. Specimens from Group 2 showed an inflammatory reaction ranging from mild to severe, with rapid resorption of the material and progressive advancement of osteoid tissue into the teflon carriers. Specimens from Group 4 showed a moderate inflammatory reaction. In 90 days, specimens from Group 1 showed a very pronounced fibrous replacement. In regard to Group 2 specimens, the tested material was solubilized and replaced by newly formed bone tissue. For Groups 3 and 5 specimens, the inflammatory reaction went from acute to moderate. In relation to Group 4 specimens, an organized bone formation process was observed.
Conclusions: Specimens from Group 2 showed higher biocompatibility, especially as compared with the specimens from Groups 3 and 5.
Keywords: Biocompatibility, calcium hydroxide, triethanolamine
|How to cite this article:|
Junior JS, Machado R, de Souza CJ, Loyola AM, Vansan LP, Antoniazzi JH. Histological analysis of the biocompatibility of calcium hydroxide associated with a new vehicle. Indian J Dent Res 2015;26:627-32
Calcium hydroxide has been recommended for use as an intracanal medicament, because of its pronounced antimicrobial activity against most of the bacterial species found in root canal infections, and also because it has a neutralizing effect on bacterial lipopolysaccharides. Moreover, it has been used mainly to help dry persistently wet canals and to reduce inflammation and pain. It also acts as a physical barrier to prevent recontamination of root canals and helps promote tissue dissolution and limit osteo-cementum-dentin resorption, thus promoting tissue restoration through mineralization. ,,,
|How to cite this URL:|
Junior JS, Machado R, de Souza CJ, Loyola AM, Vansan LP, Antoniazzi JH. Histological analysis of the biocompatibility of calcium hydroxide associated with a new vehicle. Indian J Dent Res [serial online] 2015 [cited 2019 Oct 22];26:627-32. Available from: http://www.ijdr.in/text.asp?2015/26/6/627/176929
The efficiency of calcium hydroxide as an intracanal dressing is attributed to its ionic effect, based on chemical dissociation into calcium and hydroxyl ions, which are responsible for alkalization of the medium, resulting in a pH > 11. Its high pH induces hard tissue formation through mineralization and is also responsible for its bactericidal effect. ,
Different substances have been associated with calcium hydroxide to evaluate possible changes to its antimicrobial effects, ,, biocompatibility, , pH, ,, ionic dissociation rate, and dentin diffusion. ,,,, The large number of vehicles researched and the absence of a consensus regarding the ideal vehicle are the main reasons for seeking new alternatives.
Triethanolamine is a drug that has long been used in the pharmaceutical industry because of its alkalizing potential. This characteristic enables triethanolamine to stabilize the pH of different solutions. ,,,
Therefore, the aim of this study was to make a histological evaluation of the biocompatibility of calcium hydroxide associated with triethanolamine, compared with polyethylene glycol (Calen ® ), saline solution (Calasept ® ), and olive oil (L&C paste ® ).
| Materials and Methods|| |
After approval of the study by the Research Ethics Committee of the University of São Paulo - USP/SP, 50 mice of guinea pig species were selected for this study, weighing about 800 grams each. These mice were randomly divided into five groups (n = 10) according to each vehicle to be used and were further divided into subgroups according to the analysis period (30 and 90 days) [Table 1].
The animals received general anesthesia for inoculation of the analyzed substances by intramuscular injection of 0.6 ml of ketamine (100 mg/ml, Bukwang Pharmacological Co., Seoul, Korea) mixed with acepromazine (0.5 mg/ml, Eurofarma, São Paulo, SP, Brazil).
After incision, surgical flap deflection, and exposure of the bone tissue in the anterior mandible region, standardized cavities were prepared to accommodate the teflon carriers (Polytetrafluorethylene, DuPont, HABIA, Knivsta, Sweden) 2 mm in diameter, depth, and length; 1.3 mm inner and 2 mm outer diameters; open on one side and filled with the evaluated substances.
After placing the teflon carriers on the animals, they were euthanized by chloroform inhalation (Fórmula & Ação, São Paulo, SP, Brazil) after 30 and 90 days. Their jaws were sectioned, fixed in 10% formalin solution with a sodium cacodylate buffer at 7.4 pH (Fórmula & Ação, São Paulo, SP, Brazil), and kept 48 h at 4°C for histological prefixation. Then, the plates were washed for 12 h in running water and decalcified with 5% aqueous nitric acid (Fórmula & Ação, São Paulo, SP, Brazil).
The dehydration process was performed using increasing concentrations of ethyl alcohol solution: 50%, 70%, 90%, and absolute (Fórmula & Ação, São Paulo, SP, Brazil). Afterward, the specimens were placed in paraffin to make 24 blades for each group, resulting in 120 histological semi-serial slices, about 5 μm thick, stained with hematoxylin and eosin for analysis by light microscopy.
Tissue response evaluation was based on qualitative and semi-quantitative observations of any phenomenon related to cell and tissue inflammation and repair found immediately at or at a distance from the teflon carrier/tissue interface. The type and severity of the inflammatory infiltrate were determined by two independent observers who had been calibrated for the presence or absence of (i) neutrophils, (ii) macrophages, (iii) lymphocytes, (iv) plasmocytes, (v) foreign body giant cells, (vi) dispersed material, (vii) capsules, (viii) new bone formation, (ix) tissue necrosis, and (x) bone resorption. These features were scored for intensity: (+) Absent or mild, (++) moderate, and (+++) intense. ,
| Results|| |
The quantification of cells involved in the inflammatory process, the different histopathological features [Table 2], and the description of the histological images are described below.
|Table 2: Qualitative and semi-quantitative characterization of the inflammatory process at 30 and 90 days, after intraosseous implants of the materials, based on Fédération Dentaire International and American Dental Association recommendations |
Click here to view
The specimens from Groups 1a, 3a, and 5a showed a very pronounced inflammatory response.
The specimens from Group 2a showed an inflammatory reaction ranging from mild to severe, with rapid resorption of the material and progressive advancement of osteoid tissue into the teflon carriers, the presence of cells of chronic inflammation (macrophages, lymphocytes, and giant cells), hyperemia, and dispersed material in the intimacy of the newly formed tissue [Figure 1].
|Figure 1: Light micrographs of sections of a specimen from Group 2a, showing an inflammatory reaction ranging from mild to severe, with rapid resorption of the material and progressive advancement of osteoid tissue into the teflon carriers, the presence of cells of chronic inflammation (macrophages, lymphocytes, and giant cells), hyperemia, and dispersed material in the intimacy of the newly formed tissue (a) ×110; (b) ×120; (c) ×230; (d) ×250|
Click here to view
The specimens from Group 4a showed a moderate inflammatory reaction, with a neutrophilic infiltration occupying the teflon carriers almost entirely [Figure 2].
|Figure 2: Light micrographs of sections of a specimen from Group 4a, showing moderate inflammatory reaction with neutrophilic infiltration occupying the teflon carriers almost entirely (a) ×110; (b) ×120; (c) ×230; (d) ×250|
Click here to view
In specimens from Group 1b, there was no typical fibrous capsule but very pronounced fibrous replacement [Figure 3].
|Figure 3: Light micrographs of sections of a specimen from Group 1b, showing very pronounced fibrous replacement (a) ×110; (b) ×120; (c) ×230; (d) ×250|
Click here to view
In all specimens from Group 2b, the tested material was solubilized and replaced by newly formed bone tissue. Foreign body giant cells were also seen permeating the newly formed bone interface/teflon carriers in almost the entire extension, indicating an inflammatory reaction of low intensity.
The inflammatory reaction of the specimens from Groups 3b and 5b went from acute to moderate [Figure 4].
|Figure 4: Light micrographs of sections of a specimen from Groups 3b (a and b) and 5b (c-f), showing an inflammatory reaction ranging from acute to moderate (a) ×110; (b) ×120; (c) ×110; (d) ×120; (e) ×110; (f) ×120|
Click here to view
An organized bone formation process without fibrous capsules was observed in specimens from Group 4b [Figure 5].
|Figure 5: Light micrographs of sections of a specimen from Group 4b, showing an organized bone formation process without fibrous capsules. (a) ×110; (b) ×120; (c) ×230; (d) ×250|
Click here to view
The specimens from Group 5b showed replacement of the fibrous tissue by newly formed connective tissue and reduction in the inflammatory reaction. However, there was no new bone formation.
| Discussion|| |
In view of the anatomical complexity and the resistance of some microbial species present in the root canal system, some studies have pointed to the need to use an intracanal dressing mainly to reduce this microbial contingent and its subproducts to levels that favor healing. , Since calcium hydroxide is the most widely used intracanal dressing worldwide and its effects are associated with the vehicle used, ,,,,, the lack of a consensus on the ideal vehicle warrants the search for new alternatives.
Insofar, as one of the main requirements of new materials and substances, is potentially low cytotoxic effect on tissues; ,, the aim of this study was to make a histological evaluation of the biocompatibility of calcium hydroxide associated with a new vehicle (triethanolamine), compared with traditional formulations, such as Calen ® , Calapset ® , and L&C paste ® .
In general, biocompatibility tests carried out by histological analyses aim at qualifying the inflammatory reactions occurring between tissues and evaluated materials. ,, However, these reactions are "three-dimensional processes" and a numerical rating may be dubious because of the two-dimensionality permitted by this type of analysis. For this reason, detailed descriptions and semi-quantitative analysis of inflammatory processes based on Fédération Dentaire Internationale and American Dental Association recommendations , [Table 2] were performed. These descriptions were carried out by two completely blinded evaluators, to obtain total impartiality of the results. 
The specimens from Group 2 showed less aggressive inflammatory processes than the specimens from the other groups in both study periods (30 and 90 days). This conclusion is based on the histological observations made, mainly being the resorption of the material and a marked, progressive growth of bone tissue in the teflon carriers, with different levels of maturation and specific cells of chronic inflammation (macrophages, lymphocytes, and giant cells).
Most likely, these results are associated with the chemical composition of triethanolamine, an organic compound considered both tertiary amine and tri-alcohol (C 6 H 15 NO 3 ) with a low degree of toxicity. Triethanolamine acts as a weak base, owing to the lone pair of electrons on the nitrogen atom, and has excellent potential for balancing pH when in contact with different solutions. ,,, Even though the pH of the solutions used in this study was not evaluated, triethanolamine was probably responsible for balancing the pH of the calcium hydroxide paste used as a vehicle, based on the less intense inflammatory processes observed histologically in both study periods (30 and 90 days). Similar results were observed when using saline solution as a vehicle (Group 4).
Guerreiro-Tanomaru et al.  performed a study showing that the association between calcium hydroxide and saline solution showed a progressive increase in pH values up to 14 days but remained unchanged at 21, 30, and 60 days. This may be attributed to the reduction in the available number of hydroxyl ions because of the rapid ionic dissociation that occurs when using an aqueous vehicle.  This also may explain the good results for the biocompatibility of the specimens from Groups 4a and b.
On the other hand, calcium hydroxide associated with oily vehicles, such as polyethylene glycol and olive oil (Groups 3 and 5, respectively), is capable of releasing the hydroxyl ions more slowly and causing potential irritation to the tissues for a longer period. 
Since the basic component of all pastes analyzed was calcium hydroxide, the variation in the tissue response observed may be attributed to the substances added to the pastes. The comparison of the tissue responses evaluated in this study led the authors to conclude that calcium hydroxide associated with triethanolamine was the most biocompatible association, followed by Calasept ® , Calen ® , and L&C paste ® . However, it should be borne in mind that these conclusions are based on the evaluation of tissue reactions using an animal model, the results of which cannot necessarily be extrapolated to those of apical and periapical tissues. However, it is important to conduct future evidential studies with similar methodological designs to prove the biocompatibility of calcium hydroxide associated with triethanolamine, and later studies aiming specifically at evaluating the pH of this association, and its antimicrobial effects on several types of microorganisms.
| Conclusions|| |
Calcium hydroxide paste associated with triethanolamine showed higher biocompatibility, especially compared with Calen ® and L&C paste ® .
Financial support and sponsorship
Conflicts of interest
There are no conflicts of interest.
| References|| |
Siqueira JF Jr., Lopes HP. Mechanisms of antimicrobial activity of calcium hydroxide: A critical review. Int Endod J 1999;32:361-9.
McHugh CP, Zhang P, Michalek S, Eleazer PD. pH required to kill Enterococcus faecalis in vitro
. J Endod 2004;30:218-9.
Mohammadi Z, Dummer PM Properties and applications of calcium hydroxide in endodontics and dental traumatology. Int Endod J 2011;44:697-730.
Forghani M, Mashhoor H, Rouhani A, Jafarzadeh H. Comparison of pH changes induced by calcium enriched mixture and those of calcium hydroxide in simulated root resorption defects. J Endod 2014;40:2070-3.
Ballal NV, Shavi GV, Kumar R, Kundabala M, Bhat KS. In vitro
sustained release of calcium ions and pH maintenance from different vehicles containing calcium hydroxide. J Endod 2010;36:862-6.
Lynne RE, Liewehr FR, West LA, Patton WR, Buxton TB, McPherson JC. In vitro
antimicrobial activity of various medication preparations on E. faecalis
in root canal dentin. J Endod 2003;29:187-90.
Blanscet ML, Tordik PA, Goodell GG. An agar diffusion comparison of the antimicrobial effect of calcium hydroxide at five different concentrations with three different vehicles. J Endod 2008;34:1246-8.
Lima RK, Guerreiro-Tanomaru JM, Faria-Júnior NB, Tanomaru-Filho M. Effectiveness of calcium hydroxide-based intracanal medicaments against Enterococcus faecalis
. Int Endod J 2012;45:311-6.
Nelson Filho P, Silva LA, Leonardo MR, Utrilla LS, Figueiredo F. Connective tissue responses to calcium hydroxide-based root canal medicaments. Int Endod J 1999;32:303-11.
Hauman CH, Love RM. Biocompatibility of dental materials used in contemporary endodontic therapy: A review. Part 1. Intracanal drugs and substances. Int Endod J 2003;36:75-85.
Pérez F, Franchi M, Péli JF. Effect of calcium hydroxide form and placement on root dentine pH. Int Endod J 2001;34:417-23.
Duarte MA, Midena RZ, Zeferino MA, Vivan RR, Weckwerth PH, Dos Santos F, et al.
Evaluation of pH and calcium ion release of calcium hydroxide pastes containing different substances. J Endod 2009;35:1274-7.
Beltes PG, Pissiotis E, Koulaouzidou E, Kortsaris AH. In vitro
release of hydroxyl ions from six types of calcium hydroxide nonsetting pastes. J Endod 1997;23:413-5.
Safavi K, Nakayama TA. Influence of mixing vehicle on dissociation of calcium hydroxide in solution. J Endod 2000;26:649-51.
Sevimay S, Kalayci A, Yilmaz S. In vitro
diffusion of hydroxyl ions through root dentine from various calcium hydroxide medicaments. J Oral Rehabil 2003;30:1047-51.
Guerreiro-Tanomaru JM, Chula DG, de Pontes Lima RK, Berbert FL, Tanomaru-Filho M. Release and diffusion of hydroxyl ion from calcium hydroxide-based medicaments. Dent Traumatol 2012;28:320-3.
Dlamini NN, Rajasekhar Pullabhotla VS, Revaprasadu N. Synthesis of triethanolamine (TEA) capped CdSe nanoparticles. Mater Lett 2011;65:1283-6.
Jia Z, Sun H, Gu Q. Preparation of Ag nanoparticles with triethanolamine as reducing agent and their antibacterial property. Colloids Surf A Physicochem Eng Asp 2013;419:174-9.
Nguyen AK, Gittard SD, Koroleva A, Schlie S, Gaidukeviciute A, Chichkov BN, et al.
Two-photon polymerization of polyethylene glycol diacrylate scaffolds with riboflavin and triethanolamine used as a water-soluble photoinitiator. Regen Med 2013;8:725-38.
Barbosa JA, Zoppi A, Quevedo MA, de Melo PN, de Medeiros AS, Streck L, et al.
Triethanolamine stabilization of methotrexate-ß-cyclodextrin interactions in ternary complexes. Int J Mol Sci 2014;15:17077-99.
American Dental Association. Biological Evaluation of Dental Materials. Document No. 41. New York: American Dental Association; 1982.
Federation Dentaire Internationale. Recommended Standard Practices for the Biological Evaluation of Dental Materials. Technical Report No. 9. London: Federation Dentaire Internationale; 1980.
Vera J, Siqueira JF Jr., Ricucci D, Loghin S, Fernández N, Flores B, et al.
One- versus two-visit endodontic treatment of teeth with apical periodontitis: A histobacteriologic study. J Endod 2012;38:1040-52.
Xavier AC, Martinho FC, Chung A, Oliveira LD, Jorge AO, Valera MC, et al.
One-visit versus two-visit root canal treatment: Effectiveness in the removal of endotoxins and cultivable bacteria. J Endod 2013;39:959-64.
Correa GT, Veranio GA, Silva LE, Hirata Junior R, Coil JM, Scelza MF. Cytotoxicity evaluation of two root canal sealers and a commercial calcium hydroxide paste on THP1 cell line by Trypan Blue assay. J Appl Oral Sci 2009;17:457-61.
Andolfatto C, da Silva GF, Cornélio AL, Guerreiro-Tanomaru JM, Tanomaru-Filho M, Faria G, et al.
Biocompatibility of intracanal medications based on calcium hydroxide. ISRN Dent 2012;2012:904963.
Mori GG, Rodrigues Sda S, Shibayama ST, Pomini M, do Amaral CO. Biocompatibility of a calcium hydroxide-propolis experimental paste in rat subcutaneous tissue. Braz Dent J 2014;25:104-8.
Sousa CJ, Pereira MC, Almeida RJ, Loyola AM, Silva AC, Dantas NO. Synthesis and characterization of zinc oxide nanocrystals and histologic evaluation of their biocompatibility by means of intraosseous implants. Int Endod J 2014;47:416-24.
Camargo CH, Bernardineli N, Valera MC, de Carvalho CA, de Oliveira LD, Menezes MM, et al.
Vehicle influence on calcium hydroxide pastes diffusion in human and bovine teeth. Dent Traumatol 2006;22:302-6.
Gomes BP, Ferraz CC, Vianna ME, Rosalen PL, Zaia AA, Teixeira FB, et al. In vitro
antimicrobial activity of calcium hydroxide pastes and their vehicles against selected microorganisms. Braz Dent J 2002;13:155-61.
Prof. Ricardo Machado
Department of Multidisciplinary Clinic I and II (Endodontics), Paranaense University - UNIPAR, Francisco Beltrão, Paraná
Source of Support: None, Conflict of Interest: None
[Figure 1], [Figure 2], [Figure 3], [Figure 4], [Figure 5]
[Table 1], [Table 2]
| Article Access Statistics|
| Viewed||1364 |
| Printed||27 |
| Emailed||1 |
| PDF Downloaded||86 |
| Comments ||[Add] |